Influence of force location in orthodontic shear bond strength testing. Orthodontic in vivo bond strength: comparison with in vitro results. Shear bond strength of a new fluoride-releasing orthodontic adhesive. Comparison of bond strength between a conventional resin adhesive and a resin-modified glass ionomer adhesive: an in vitro and in vivo study. The influence of adding modified zirconium oxide-titanium dioxide nano-particles on mechanical properties of orthodontic adhesive: an in vitro study Bond strength comparison of moisture-insensitive primers. Argon laser vs conventional visible light-cured orthodontic bracket bonding: an in-vivo and in-vitro study. Shear bond strength comparison between two orthodontic adhesives and self-ligating and conventional brackets. Effects on shear bond strength and the enamel surface with an enamel bonding agent. Effect of changing a test parameter on the shear bond strength of orthodontic brackets. Comparison of bond strength between orthodontic brackets bonded with halogen and plasma arc curing lights: an in-vitro and in-vivo study. Effect of cyclic impact load on shear bond strength of zirconium dioxide ceramics. Comparison of bond strength of three adhesives: composite resin, hybrid GIC, and glass-filled GIC. Influence of surface treatment and simulated aging on bond strengths of luting agents to zirconia. A new one-step dental flowable composite for orthodontic use: an in vitro bond strength study. New protective polish effects on shear bond strength of brackets. The influence of orthodontic bracket base design on shear bond strength. Can previously bleached teeth be bonded safely? Casein Phosphopeptide-Amorphous Calcium Phosphate and Shear Bond Strength of Adhesives to Primary Teeth Enamel Bonding strength to two different surfaces of dentin under simulated pulpal pressure. The effect of different power outputs of carbon dioxide laser on bonding between zirconia ceramic surface and resin cement In vitro bond strengths of resin modified glass ionomer cements and composite resin self-cure adhesives: introduction of an adhesive system with increased bond strength and inhibition of decalcification. In vitro evaluation of shear bond strength and microleakage of different pit and fissure sealants
OBJECTIVE The purpose of the present study was to analyze the influence of debonding force location in shear bond strength testing of orthodontic brackets in vitro . METHODS Ninety extracted permanent bovine m and ibular incisors were r and omly divided into 3 groups of 30 specimens each . Teeth were bonded with stainless steel orthodontic brackets . Enamel surfaces were etched with 37 % phosphoric acid for 30s and bonded with a composite adhesive .  Debonding force measurements were performed with a universal testing machine . Location of the debonding force was : bracket base ( group A ) , ligature groove ( group B ) , occlusal bracket wings ( group C ) . RESULTS Mean shear bond strength measurements were as follows : 22.70(4.23)MPa ( group A ) , 11.52(2.74)MPa ( group B ) , 9.44(2.96)MPa ( group C ) . Analysis of variance indicated that there were significant differences in shear bond strength . Post-hoc Tukey tests showed that bond strength measurements of group A were significantly different from those of groups B and C. The adhesive remnant index also showed significant differences and ranged from a mean of 1.53 in group A to a mean of 2.10 in group C. SIGNIFICANCE Debonding force location had a significant influence on shear bond strength measurements and bond failure pattern , indicating that this parameter needs to be taken into consideration for inter study comparison of in vitro results The purpose of the present study was to test a new in vivo debonding device and compare in vivo bond strengths recorded by this device with in vitro bond strengths recorded by a universal testing machine such as the Instron . For the in vitro part of the study , 60 extracted premolar teeth were divided into 2 groups of 30 each . Both groups of 30 teeth had 3 M Unitek Victory Twin brackets , precoated with Transbond XT composite resin , bonded to them . Shear bond strength tests were carried out in vitro using the universal testing machine on one group of 30 teeth while the debonding device was used on the other group of 30 teeth . The mean shear bond strength of the group debonded using the universal machine was 11.02 MPa and that of the group debonded with the debonding device was 12.82 MPa . For the in vivo part of the study , 8 patients r and omly assigned to the research clinician from patients in The University of Alabama School of Dentistry , Department of Orthodontics , had a total of 60 premolar teeth bonded with 3 M Unitek Victory Twin brackets . Following comprehensive orthodontic treatment ( average time of 23 months ) , shear bond strength tests were carried out using the debonding device , which can measure debonding forces in vivo . The mean shear bond strength recorded in vivo was 5.47 MPa . Statistically significant differences were found between all 3 groups tested . The results appear to indicate that mean bond strengths recorded in vivo following comprehensive orthodontic treatment are significantly lower than bond strengths recorded in vitro This study evaluated the shear bond strength of stainless steel brackets bonded to enamel with a new fluoride-releasing orthodontic adhesive system . A total of 140 extracted human bicuspids were r and omly divided into four groups . Group I ( Transbond XT ) was a control group in which enamel was etched with phosphoric acid . For the remaining groups , enamel was conditioned with a self-etching primer ( SEP ) : Group II ( Transbond Plus ) , Group III ( BeautyOrtho Bond ) , and Group IV ( BeautyOrtho Bond + Salivatect ) . Stainless steel brackets were bonded to all tooth sample s. After which , the sample s were stored , thermocycled , tested , and statistically analyzed . Besides bond strength evaluation , the adhesive remnant index ( ARI ) was also evaluated . The shear bond strengths of Groups II , III , and IV were significantly lower than Group I , and Group II was significantly greater than that of Group III . Concerning ARI scores , no significant differences were found between the groups . Further , no enamel fracture was observed during shear bond test with the new SEP . In conclusion , when enamel was conditioned with the new SEP , the mean values of shear bond strength yielded were lower than when it was etched with 37 % phosphoric acid . Nonetheless , these mean values were higher than the average suggested by Reynolds as optimum for clinical treatment The objectives of this study were ( 1 ) to compare the in vivo survival rates of orthodontic brackets bonded with a resin-modified glass ionomer adhesive ( Fuji Ortho LC ; GC America , Alsip , Ill ) after conditioning with 10 % polyacrylic acid and a conventional resin adhesive ( Light Bond ; Reliance Orthodontic Products , Itasca , Ill ) bonded with 37 % phosphoric acid , ( 2 ) to compare the in vitro bond shear/peel bond strength between the 2 adhesives , ( 3 ) to determine the mode of bracket failure in the in vivo and in vitro tests according to the adhesive remnant index ( ARI ) , and ( 4 ) to compare the changes in surface morphology of enamel surface after etching or conditioning with 10 % polyacrylic acid , with scanning electron microscopy . In the in vitro study , 50 extracted premolars were r and omly divided into 4 groups : brackets bonded with Fuji Ortho LC or Light Bond adhesive that were debonded after either 30 minutes or 24 hours . Bond strengths were determined with a testing machine at a crosshead speed of 1 mm/min . Data were analyzed with analysis of variance and a paired Student t test . The in vivo study consisted of 398 teeth that were r and omly bonded with Fuji Ortho LC or Light Bond adhesive in 22 subjects with the split-mouth technique . Bracket survival rates and distribution were followed for 1.3 years . Data were analyzed with Kaplan-Meier product-limit estimates of survivorship function . The in vitro study results showed significant differences ( P < .05 ) among the adhesives and the debond times . Light Bond had significantly greater bond strengths than Fuji Ortho LC at 24 hours ( 18.46 + /- 2.95 MPa vs 9.56 + /- 1.85 MPa ) and 30 minutes ( 16.19 + /- 2.04 MPa vs 6.93 + /- 1.93 MPa ) . Mean ARI scores showed that Fuji Ortho LC had significantly greater incidences of enamel/adhesive failure than Light Bond adhesive ( 4.9 vs 4.1 ) . For the in vivo study , no significant differences in failure rate , sex , or location in dental arch or ARI ratings were found between the 2 adhesives . These results suggest that , compared with conventional resin , brackets bonded with resin-modified glass ionomer adhesive had significantly less shear bond strength in vitro . However , similar survival rates of the 2 material s studied after 1.3 years indicate that resin-reinforced glass ionomers can provide adequate bond strengths clinical ly . The weaker chemical bonding between the adhesive and the enamel might make it easier for clinicians to clean up adhesives on the enamel surface after debonding Background The purpose of this in-vitro study was to examine the effect of incorporating different concentrations of Zirconium oxide-Titanium dioxide ( ZrO2-TiO2 ) nanoparticles , which can have antibacterial properties , on the mechanical properties of an orthodontic adhesive . Methods ZrO2-TiO2 ( Zirconium oxide , HWNANO , Hongwu International Group Ltd , China ) -Titanium dioxide , Nanoshell , USA ) nanopowder were incorporated into orthodontic adhesive ( Transbond XT , 3 M Unitek , Monrovia , USA ) with different concentrations ( 0.5 % weight nonofiller and 1 % weight nanofiller ) . The size of nanoparticle was 70–80 nm for ZrO2 and less than 50 nm for TiO2 . For measuring the shear bond strength of the three groups of orthodontic adhesives [ Transbond ( control ) , Transbond mixed with 0.5 % weight ZrO2-TiO2 , and Transbond mixed with 1 % weight ZrO2-TiO2 ] , 30 freshly extracted human first premolars were used and bonded with stainless steel metal brackets ( Dentaurum ® , Discovery ® , Deutschl and ) , using the 3 orthodontic adhesives and 3 M Unitek ; Transbond TM Plus Self-Etching Primer ( 10 sample s in each group ) . The recorded values of compressive strength and tensile strength ( measured separately on 10 sample s of orthodontic adhesives ( add the 3 D size of sample , light cured for 40 s on both sides ) of each orthodontic adhesives ) , as well as the shear bond strength in Mega Pascal unit ( MPa ) were collected and exposed to one-way analysis of variance ( ANOVA ) and Tukey ’s post-hoc tests . Results orthodontic adhesive with 1 % weight ZrO2-TiO2 showed the highest mean compressive ( 73.42 ± 1.55 MPa , p : 0.003 , F : 12.74 ) , tensile strength ( 8.65 ± 0.74 MPa , p : 0.001 , F : 68.20 ) , and shear bond strength ( 20.05 ± 0.2 MPa , p : 0.001 , F : 0.17 ) . Conclusions Adding ZrO2-TiO2 nanoparticle to orthodontic adhesive increased compressive strength , tensile strength , and shear bond strength in vitro , but in vivo studies and r and omized clinical trials are needed to vali date the present findings The objective of this in vitro bonding study was to evaluate the effectiveness of 2 moisture-insensitive primers , Assure ( Reliance Orthodontic Products , Itasca , Ill ) and MIP ( 3 M Unitek , Monrovia , Calif ) compared with a control hydrophobic primer , Transbond XT ( 3 M Unitek ) . Six groups of 40 premolars were acid etched and bonded using metal orthodontic brackets with the following in vitro protocol s : ( 1 ) Transbond XT primer and adhesive applied to a noncontaminated surface ; ( 2 ) Assure primer applied after saliva contamination ; ( 3 ) MIP primer applied after saliva contamination ; ( 4 ) Assure primer reapplied after saliva contamination ; ( 5 ) MIP reapplied after saliva contamination ; and ( 6 ) Assure adhesive applied after saliva contamination of the primer . All bonded specimens were stored in deionized water at 37 degrees C for 30 days and thermocycled for 24 hours before debonding . Brackets were debonded using a shear-peel load on a testing machine , bond strength was measured in megapascals , and bond failure was analyzed by using the adhesive remnant index . In vitro shear-peel bond strengths were acceptable for all groups , and the bond strengths for Assure and MIP were not significantly affected by saliva contamination . The mean shear-peel bond strength of the control ( 14.82 MPa ) was significantly higher ( P < .001 ) than the contaminated groups with the exception of MIP group 5 ( 14.02 MPa ) . The values of the Assure primer and adhesive were less than the MIP primer and its respective adhesive ; however , the hydrophilic Assure adhesive resin applied to a saliva-contaminated surface had acceptable bond strength . Bond failure analysis ( adhesive remnant index ) mainly showed adhesive bond failures . An increased frequency of enamel fractures at debond was noted , with the control group ( 1 ) and the MIP groups ( 3 and 5 ) having 22.5 % , 12.5 % , and 15 % , respectively . The Assure groups had no enamel fractures INTRODUCTION Many advantages of argon lasers have been reported , including high-speed orthodontic adhesive curing and less enamel demineralization . The purpose of this study was to compare bond strengths after curing with the argon laser ( 10 seconds ) and the conventional curing light ( 40 seconds ) in vivo and in vitro . METHODS Four premolars from each of 23 volunteers were r and omly assigned to either the argon laser group or the conventional light group for the in-vivo study . Shear bond strengths were measured after 14 days with custom- design ed debonding pliers . In-vitro bond strengths were measured by using 4 premolars from each of 25 volunteers .  Shear bond strength was measured after 14 days of thermocycling with the same protocol as the in-vivo study . Adhesive remnant index scores ( ARI ) were determined . RESULTS No significant differences were found in bond strengths according to curing method , dental arch , or sex . In-vivo results were significantly lower ( P < .05 ) than in-vitro results . A significant ( P < .05 ) difference in ARI scores between the curing methods was determined ; no significant correlation between mean bond strengths and ARI scores was determined . CONCLUSIONS Bond strength for argon laser curing is comparable to conventional light curing and is sufficient for clinical applications . Although the argon laser left more adhesive on the tooth surfaces on debonding , there was no increase in enamel surface fractures OBJECTIVE To evaluate and compare the shear bond strengths of two adhesives using two types of brackets : a conventional and a self-ligating bracket system . MATERIAL S AND METHODS Sixty extracted human premolars were collected . The premolars were r and omly divided into three groups of 20 teeth . All three groups were direct bonded . Groups 1 and 2 used light-cured adhesive and primer ( Transbond XT ) with a conventional ( Orthos ) and a self-ligating bracket ( Damon 2 ) , respectively . Group 3 used a light-cured primer ( Orthosolo ) and a light-cured adhesive ( Blūgloo ) with a self-ligating bracket ( Damon 2 ) . The specimens were stored in distilled water at 37 degrees C for 40 + /- 2 hours , after which they were debonded and inspected for Adhesive Remnant Index ( ARI ) scoring . RESULTS The mean shear bond strength was 15.2 MPa for group 1 , 23.2 MPa for group 2 , and 24.8 MPa for group 3 . A one-way analysis of variance and post hoc Tukey test showed significant differences in bond strength ( P < .001 ) between group 1 and groups 2 and 3 but no significant difference ( P > .05 ) between groups 2 and 3 . A Weibull analysis demonstrated that all three groups provided sufficient bond strength with over 90 % survival rate at normal masticatory and orthodontic force levels . A Kruskal-Wallis test showed no significant difference ( P > .05 ) in ARI scores among all three groups . CONCLUSIONS All three groups demonstrated clinical ly acceptable bond strength . The Damon 2 self-ligating bracket exhibited satisfactory in vitro bond strength with both adhesive systems used INTRODUCTION The purpose of this study was to evaluate the shear bond strength of orthodontic brackets and the effect of an enamel bonding agent ( EBA ) on enamel surface after debonding . METHODS Seventy-five extracted maxillary premolars were collected and r and omly divided into 3 groups of 25 . The enamel cracks were surveyed with a stereomicroscope . In the first group , 1 layer of EBA was applied before the adhesive resin . In the second group , 2 layers of EBA were used ; in the third group , no EBA was used . Bonding was followed by incubation for 48 hours at 37 degrees C and thermocycling for 1000 cycles . Debonding was performed with a shear force . The surfaces of the teeth were evaluated , and the length , depth , direction of cracks , and adhesive remnants on the enamel surface were recorded . Data were analyzed by using analysis of variance and paired sample s t tests . RESULTS There were no significant differences between the shear bond strengths ( P = 0.341 ) of the 3 groups , or in the direction , length , and depth of the cracks before and after debonding ( P > 0.05 ) . There was a significant increase in the number of cracks after debonding in the 3 groups ( P < 0.05 ) . The evaluation of adhesive remaining on the surface of the teeth indicated that most bond failures occurred at the resin-bracket interface . CONCLUSIONS The use of EBA does not enhance bond strength or provide greater protection to the enamel surface during debonding The purpose of this study was to determine the effect of changing the crosshead speed of the testing machine on the shear bond strength of orthodontic brackets to enamel while st and ardizing all the other variables . Forty freshly extracted human molars were bonded using the Transbond XT adhesive system ( 3 M Unitek , Monrovia , Calif ) . The teeth were r and omly divided into two groups . In group I , the shear bond strength was measured at a crosshead speed of 5.0 mm/min , and in group II the shear bond strength was measured at a crosshead speed of 0.5 mm/ min . Within half an hour from the initial bonding of each tooth , an occlusogingival load was applied to the bracket , producing a shear force at the bracket-tooth interface . This was accomplished by using the flattened end of a steel rod attached to the crosshead of a Universal Test Machine ( Zwick GmbH & Co , Ulm , Germany ) . The t-test results ( t = 2.71 ) indicated that there was a significant difference ( P = .014 ) in the shear bond strengths between the group tested at a crosshead speed of 5.0 mm/min and the group tested at a crosshead speed of 0.5 mm/min . The mean shear bond strengths for the two groups were 7.0 + /- 4.6 MPa and 12.2 + /- 4.0 MPa , respectively . These findings indicated that it is important to identify the parameters included in shear bond testing in order to enable meaningful comparisons of the performance of different material INTRODUCTION This study assessed in-vitro shear bond strength and in-vivo survival rate of orthodontic brackets bonded with either a halogen  or a plasma arc light . METHODS Ninety extracted premolars were divided into 6 groups of 15 . Stainless steel brackets were bonded to the teeth by using either a halogen light with a 20-second curing time or a plasma arc light with a 2- , 6- , or 10-second curing time . Brackets were debonded either within 30 minutes of bonding or after thermocycling for 24 hours . Bond strengths were tested on a testing machine at a crosshead speed of 1 mm/minute . The bracket failure interface was measured with a modified adhesive remnant index score . Data were analyzed by using ANOVA and Tukey-Kramer multiple comparison tests . For the in-vivo study , a split-arch design was used to determine the bracket-failure rate and distribution in 25 patients . The patients were followed for a mean period of 1.1 years ( 386 days ) . Survival analysis was carried out to compare the failure rates of the 2 techniques . RESULTS No significant differences in bond strengths were found 30 minutes after bonding between the halogen light ( 13.6 + /- 3.8 MPa ) and the plasma arc light with 2- , 6- , or 10-second curing times ( 9.6 + /- 2.9 , 14.2 + /- 4.6 , 16.0 + /- 3.0 MPa , respectively ) . Similar bond strengths were also found between the halogen light with a 20-second ( 16.1 + /- 3.6 MPa ) curing time and plasma arc light with 6 seconds ( 18.2 + /- 4.6 MPa ) of curing time after 24 hours of thermocycling . For the in-vivo study , no significant difference was found in bracket failure rates between the 2 light sources ( 4.9 % in both groups ) . No significant differences were found between ARI scores for the halogen light and the plasma arc light at either 30 minutes or 24 hours after debonding . CONCLUSIONS These results indicate that the plasma arc light with a 6-second curing time can produce similar bond strength and bracket-failure rates as the halogen light that requires a longer curing time PURPOSE To investigate the influence of cyclic impact load and the number of load cycles on compressive shear bond strength under the three different cements . MATERIAL S AND METHODS The following material s were used : Super Bond C&B ( SB ) and Panavia Fluoro Cement ( PF ) as adhesive resin cements , Fuji Luting ( FL ) as a resin-modified glass-ionomer cement , and zirconium dioxide ceramics as adherend . Before the shear bond test , three different impact loading conditions ( compressive direction , shear direction , and no impact ) and the number of load cycles ( 1 to 106 cycles ) , were performed . A total of 189 specimens ( n = 3/group ) were r and omly assigned to groups and tested . A cyclic impact test was performed by applying a load of 98N at a distance of 40 mm and a loading cycle frequency of 1 Hz . All results were statistically analyzed with two-way ANOVA and Tukey 's multiple comparison test . RESULTS Shear bond strengths of SB , PF , and FL subjected to no cyclic impact load were 21.6 to 53.8 MPa in SB , 27.0 to 63.6 MPa in PF , and 20.0 to 35.9 MPa in FL . The shear bond strength of SB and PF increased to a certain degree from one to 105 cycles , while FL did likewise from one to 104 cycles . CONCLUSION The shear bond strengths of SB , PF , and FL were greatest without cyclic impact , followed by compressive and then shear cyclic impact The objective of this study was to compare 3  orthodontic adhesives  in the areas of shear-peel bond strength , location of adhesive failure , and extent of enamel cracking before bonding and after debonding of orthodontic brackets . The adhesives included a composite resin control ( Transbond XT ; 3M/Unitek , St Paul , Minn ) , a resin-modified glass ionomer cement ( Fuji Ortho LC ; GC America Corp , Alsip , Ill ) , and a polyacid-modified composite resin under dry and saliva-contaminated conditions ( Assure ; Reliance Orthodontic Products Inc , Itasca , Ill ) . Metal brackets were bonded to the buccal surfaces of 160 ( 4 groups of 40 ) human premolars . The bonded teeth were stored in deionized water at 37 degrees C for 30 days and thermocycled for 24 hours before debonding with a Universal Instron ( Instron Corp , Canton , Mass ) testing machine . The extent of cracking in the buccal surfaces was evaluated under 16x magnification before bonding and after debonding . Although the bond strength of the composite resin control ( 20.19 MPa ) was significantly greater ( P < .05 ) than that of the adhesives in the other groups , clinical ly acceptable shear-peel bond strengths were found for all adhesives ( Fuji Ortho LC = 13.57 MPa , Assure-dry = 10.74 MPa , Assure-wet = 10.99 MPa ) . The bond strength for the Assure adhesive was not significantly affected by saliva contamination . The sample of extracted premolars used in this study displayed a greater frequency of buccal surface enamel cracking ( 46.7 % ) than that reported in the literature for in vivo premolars ( 7.8%-10.2 % ) , which was possibly due to the extraction process . The frequency of enamel cracking in a subset of this sample ( n = 34 ) increased from 46.4 % at prebonding to 62.4 % at postdebonding as a result of the forces of debonding OBJECTIVE To evaluate short- and long-term shear bond strengths of 4 luting agents to zirconia following different surface treatments . METHOD AND MATERIAL S A total of 320 ceramic specimens fabricated from a commercial zirconium oxide ceramic ( Lava ) were r and omly divided into 4 groups : left untreated ( NOT ) , airborne-particle abraded ( SND ) , Rocatec tribochemical silica/silane coated ( ROC ) , or ground and polished ( GRD ) . Resin composite cylinders were bonded to the zirconia specimens with resin composite luting agent RelyX ARC ( ARC ) , universal adhesive resin composite RelyX Unicem ( UNI ) , adhesive-phosphate-monomer-containing resin composite Panavia F ( PAN ) , or the hybrid glass-ionomer cement RelyX Luting ( LUT ) .  Subgroups of 10 specimens were stored in distilled water ( 37 degrees C ) for 3 days ( ST ) or stored for 180 days and thermocycled for 12,000 cycles ( LT/TC ) before shear bond strength was tested . Statistical analyses included Kruskal-Wallis and Wilcoxon 2- sample rank sum test ( alpha = .01 ) . RESULTS Short-term shear bond strengths were higher with ROC than with SND , which were both greater than GRD or NOT . UNI revealed higher shear bond strengths than PAN , ARC , and LUT . LT/TC significantly decreased shear bond strength values . GRD and NOT produced the lowest shear bond strengths . SND and ROC significantly increased bond strength . ROC generally yielded the highest long-term shear bond strength , especially with UNI , PAN , or ARC . These were similar to SND and PAN , which revealed the highest long-term shear bond strengths . CONCLUSIONS Surface treatment , luting agent , and storage conditions significantly influence shear bond strengths to zirconia . Artificial aging significantly reduces shear bond strengths . Airborne-particle abrasion combined with a resin composite containing adhesive phosphate monomers or tribochemical silica/silane coating combined with any of the tested resin composite luting agents provides superior long-term shear bond strength values A new flowable composite , Denfil Flow , has shown an acceptable shear bond strength for bonding orthodontic brackets , when used with an intermediate , unfilled , low-viscosity resin . According to the manufacturer , it also shows a good viscosity for use with no preliminary adhesive . This could reduce the total time of bonding procedure while maintaining clinical ly useful bond strength . The aim of the current research was to assess this property . Eighty extracted human premolars were r and omly divided into four equal groups . Stainless steel brackets were bonded to etched enamel using ( 1 ) Denfil Flow , ( 2 ) a traditional flowable composite ( Dyract Flow ) , ( 3 ) Denfil Flow composite resin and an intermediate liquid resin , and ( 4 ) Transbond XT adhesive . Debonding was performed with a shearing force . The residual adhesive on the enamel surface was evaluated using the adhesive remnant index . The bond strength of Denfil Flow ( 34.8 MPa ) showed no significant difference with the other control groups and was clinical ly acceptable . Denfil Flow and Dyract Flow tended to display cohesive failure within the adhesive . Denfil Flow can be used without liquid resin to reduce the bonding procedure time while maintaining acceptable bond strength . Further studies are required to evaluate the enamel surface of the teeth after the same polishing procedure in the four groups One of the solutions for the problem of white spot lesions has been the application of a polymer coating to the labial enamel surface . The aim of this study is to find out whether the liquid polish BisCover affects the bond strength of brackets bonded with a light-cured system ( Transbond XT ) and a no-mix system ( Unite ) . St and ard stainless steel premolar brackets were bonded to 100 permanent human premolars r and omly divided into five equal groups . Two different enamel surface conditions were studied : dry and varnished with BisCover . For each enamel surface condition , two orthodontic adhesive systems were used : a light-cured system ( Transbond XT ) and a no-mix system ( Unite ) . All teeth were conditioned with 37 % phosphoric acid for 30 seconds , followed by thorough washing and drying . The teeth in groups 1 and 2 were bonded with Transbond XT and Unite , respectively . For groups 3 , 4 , and 5 , a thin layer of BisCover was applied to the etched enamel with a brush and light cured for 15 seconds . In group 3 , a thin layer of Transbond XT primer was applied , whereas in group 5 , no additional primer was used on BisCover . In groups 3 and 5 , the brackets were bonded with Transbond XT adhesive resin . Group 4 was bonded with no-mix Unite . Shear forces were applied to the sample s by a Zwick Universal test machine , and bond strengths measured in megapascals . The results revealed that shear bond strengths of the groups did not differ significantly from each other Many bracket base design s and adhesive material s are in clinical use today . Bases have evolved from perforated metal bases to the present foil mesh bases , and treatments range from none , to spraying metal alloy onto the base , to the most common treatment of microetching . The purpose of this study was to determine the effect of orthodontic bracket base design on mean shear bond strength 1 hour or 24 hours after bonding . For each time group , 12 specimens of 6 types of metal brackets were bonded to bovine incisors with Transbond XT ( 3 M Unitek , Monrovia , Calif ) light-cured composite resin . Brackets were debonded 1 hour or 24 hours later , and the shear bond strength was recorded . Six debonded brackets of each type from each time group were selected at r and om and s and blasted . All the teeth were cleaned , and half were rebonded with used brackets , and half were rebonded with new brackets . Bond strength was measured again , 1 hour or 24 hours later . Representative specimens were inspected under the scanning electron microscope . Bracket base design significantly affected mean shear bond strength . Speed ( 60-gauge , microetched foil-mesh base ; Strite Industries , Cambridge , Ontario , Canada ) had the highest bond strength at 1 hour ; followed by Time ( machined , integral , microetched base with mechanical undercuts ; American Orthodontics , Sheboygan , Wis ) ; American Master Series ( 80-gauge foil-mesh base ; American Orthodontics ) ; Ovation Roth ( 80-gauge layered onto 150-gauge , microetched foil-mesh base ; GAC , Central Islip , NY ) ; Orthos Optimesh XRT ( 100-gauge microetched foil-mesh base ; Ormco , Orange , Calif ) ; and , finally , the nickel-free brackets ( injection molded , 100-gauge , microetched , foil-mesh base ; World Class Technology , McMinnville , Ore ) . The 24-hour results were similar except that Time had the highest mean shear bond strength ( ANOVA , P < .05 ) . Chairside s and blasting significantly affected the 1-hour , but not the 24-hour , mean shear bond strengths ( ANOVA , P < .05 ) . S and blasting appears to be an effective method of cleaning bracket bases before rebonding The purpose of our study was to determine the effect of a 35 % hydrogen peroxide bleaching agent on the shear bond strength of metallic orthodontic brackets . Sixty premolars were r and omly divided into 3 groups of 20 each . Teeth in group A were etched with 37 % phosphoric acid before bonding metallic premolar brackets . Teeth in the other 2 groups were bleached with a 35 % hydrogen peroxide in-office bleaching agent according to the manufacturer 's recommendations . Twenty bleached teeth ( group B ) were bonded immediately , and the other 20 ( group C ) were stored in artificial saliva for 30 days before bonding . Shear bond strength of these brackets was measured on a universal testing machine and recorded in MPa . Adhesive remnant index ( ARI ) scores were determined after the brackets failed . Data were analyzed with analysis of variance ( ANOVA ) and chi-square tests . The shear bond strength values of groups A , B , and C were 12.9 + /- 3.4 , 12.0 + /- 4.6 , and 14.8 + /- 4.0 MPa , respectively . Results of ANOVA showed no statistically significant differences in shear bond strengths between groups ( P > .05 ) . ARI scores were significantly different in all groups . The unbleached group 's failures were primarily at the bracket/adhesive interface , whereas the bleached groups either showed cohesive failures within the adhesive or failed at the adhesive/enamel interface . The results of this study suggest that office bleaching with hydrogen peroxide does not adversely affect the bond strengths of brackets bonded immediately after bleaching or 30 days after bleaching , even though bleaching can result in differences in the failure site Background : CPP-ACP ( Phosphopeptide-Amorphous Calcium Phosphate ) has an important role in caries prevention in pediatric patients . This study was done , because of the great use of CPP-ACP and the need for restoration for teeth treated with CPP-ACP as well as the importance of shear bond strength of adhesives in the success of restorations . Objectives : This study aim ed to evaluate the effect of casein phosphopeptide-amorphous calcium phosphate ( CPP-ACP ) on shear bond strength of dental adhesives to enamel of primary teeth molars . Material s and Methods : This in vitro study was conducted on 180 extracted primary molars . They were r and omly divided into 6 groups and each group was divided into 2 subgroups ( treated with CPP-ACP and untreated ) . In subgroups with CPP-ACP , enamel was treated with CPP-ACP paste 1 h/d for 5 days . Types of adhesives that were evaluated in this study were Tetric N-Bond , AdheSE , AdheSE One F , single Bond 2 , SE Bond , and Adper Prompt L-Pop . Shear bond strength was tested with a universal testing machine and mode of failure was evaluated under stereomicroscope . Data were analyzed by T test , 2-way analysis of variance ( ANOVA ) , Tukey and Fisher exact test using SPSS18 . P < 0.05 was considered as significance level . Results : Shear bond strengths of different adhesive systems to enamel of primary teeth treated and untreated with CPP-ACP showed no significant difference ( P > 0.05 ) . Mode of failure in all groups regardless of CPP-ACP administration was mainly adhesive type . Our results indicated that CPP-ACP did not affect shear bond strength of studied adhesives to primary teeth enamel . Conclusions : To have a successful and durable composite restoration , having a high strength bonding is essential . Considering the wide use of CPP-ACP in preventing tooth decay and the role of adhesive shear bond strength ( SBS ) in success of composite restoration , we conducted the present study to evaluate the effect of CPP-ACP on the SBS of adhesives to primary teeth enamel PURPOSE The purpose of this in vitro study was to measure and compare the in vitro shear bond strengths ( SBS ) of the following dentin bonding systems to different dentin surfaces under simulated pulpal pressure : Liner Bond 2 ( self-etching ) ( LB2 ) , Liner Bond 2V ( self-etching ) ( LB2V ) , Opti Bond Solo ( single component ) ( OBS ) , Fuji Bond LC ( filled ) ( FBLC ) , Prime & Bond 2 - 1 ( single component ) ( P&B2 - 1 ) , and Solid Bond ( total etching ) ( SB ) . MATERIAL S AND METHODS Occlusal and buccal surfaces of 60 extracted human molars were prepared to expose the dentin bonding surface . After being wet ground with 600-grit abrasive papers , teeth were r and omly assigned to 6 equal groups of 10 each . The dentin surfaces were treated with the bonding systems mentioned above , and resin composite cylinders ( Clearfil AP-X ) were built up under simulated pulpal pressure when diluted bovine serum was used as the pulpal fluid . After one day of storage in 37 degrees C water , the specimens were shear tested to failure on an Instron machine . RESULTS The data were statistically analyzed with the Student 's t-test and a post hoc Tukey test . Comparing buccal surfaces , the post hoc Tukey test indicated no significant differences among all the test groups ( p > 0.05 ) . On occlusal surfaces , the post hoc Tukey test indicated significant differences among the tested groups ( p < 0.05 ) . The Student 's t test revealed significant differences between the occlusal and buccal shear bond strength values in LB 2 , LB2V , and SB groups ( p < 0.05 ) . CONCLUSION The strength of adhesion to dentin depends upon both the adhesive system used - with self-etching systems tending to show higher bond strengths than the other material s tested - and the location of the dentin , with significantly higher SBS being found on buccal surfaces in 3 of the 7 tested bonding systems Abstract Objective . The purpose of this in vitro study was to evaluate the influence of different power outputs of a carbon dioxide ( CO2 ) laser on shear bond strength of resin cement to zirconium dioxide-based ceramic . Material s and methods . Fifty zirconium dioxide core specimens ( 10 mm diameter and 2 mm thickness ) were produced and they were embedded in the centers of auto-polymerizing acrylic resin blocks . Ten specimens served as control and no surface treatment was applied . Subsequently specimens were r and omly divided into four groups , each containing 10 specimens for surface treatment with CO2 laser with different output power ; laser treated with 2 W ( Group 2 W ) , 3 W ( Group 3 W ) , 4 W ( Group 4 W ) and finally 5 W ( Group 5 W ) . Fifty composite resin discs were fabricated and cemented with adhesive resin cement to the specimen surfaces . A universal test machine was used for shear bond strength test at a crosshead speed 1 mm/min . Data were statistically analyzed by one-way analyses of variance ( ANOVA ) with Post-Hoc Tukey tests ( α = 0.05 ) . Results . It was found that the shear bond strength values were affected by power outputs of laser ( p < 0.05 ) . Highest shear bond strength values were obtained with group 2 W ( 21.0 ± 2.7 ) . Lowest values were obtained with group 5 W ( 14.4 ± 1.6 ) . Conclusion . The current study revealed that there was a relationship between laser output power and shear bond strength for zirconium dioxide ceramics . However , output power of the laser and the energy level is a critical factor on micromechanical retention This study evaluated the shear bond strength and adhesive remnant index of 5 self-cure adhesives to comparatively evaluate a new adhesive system . Extracted human incisors were r and omly divided into 7 test groups of 20 each .  Incisor mesh-backed brackets were bonded to the tooth specimens in each group with their respective adhesive according to the manufacturer 's instructions . The specimens were thermocycled for 2 weeks at temperatures from 5 degrees to 55 degrees C to simulate oral conditions and debonded using an Instron machine . Acceptable bond strength parameters were present with the Contacto No-Mix ( composite resin containing glass ionomer 8.75 MPa ) and Fuji Ortho SC with acid conditioning ( 6.98 MPa ) . Contacto No-Mix had a higher bond strength ( 11.2 MPa ) when microetching and Megabond were employed than when these adjuncts were not employed . When FUJI Ortho SC specimens were conditioned with polyacrylic acid , they showed a higher bond strength ( 6.98 MPa ) than when bonded to unetched teeth ( 5.41 MPa ) . In test 3 , EXPT-fluoride adhesive ( AF ) demonstrated a higher bond strength ( 13.44 MPa ) than both resin composite Contacto No-Mix ( 8.8 MPa , GAC 7.4 MPa ) and FUJI Ortho SC ( 5.41 MPa ) . Expt AF ( Test 3 ) and Concise had equal bond strengths , however , the former can potentially release fluoride from the glass ionomer . Although the Aim and Objectives : Fissure caries is most common in children due to deep pit and fissures . Pit and fissure areas on the occlusal surface of the teeth make them susceptible to dental caries , which need to be prevented or restored . Fissures sealant reduces the risk of occlusal caries . The present study was done to evaluate microleakage and shear bond strength of various fissure sealants . Material s and Methods : Thirty-six extracted molars were r and omly allocated equally ( n = 12 ) into three groups with three different sealants to evaluate shear bond strength and microleakage at sealant space . The shear bond strengths was evaluated with one-way analysis of variance and microleakage by Kruskal-Wallis nonparametric test using the Statistical Package for the Social Sciences version 18.0 ( Chicago : SPSS Inc , 2009 ) . Results : Tetric flow ( 16.8 MPa ) recorded the highest shear bond strength and the difference was statistically significant with enamel loc ( 12.8 MPa ) . There was no statistically significant difference in relation to microleakage ( P > 0.05 ) in the tested groups . Conclusions : Tetric flow recorded the highest shear bond strength and the difference was statistically significant with enamel loc . However , there was no statistically significant difference among the groups regarding microleakage
Many studies on in-vitro orthodontic bond strength fail to report test conditions that could significantly affect their outcomes
INTRODUCTION The aims of this study were to systematic ally review the available literature regarding in-vitro orthodontic shear bond strength testing and to analyze the influence of test conditions on bond strength .